 to be weak, accordingly, the correlation length, or the characteristic size of the pair is $l_{corr}>>n^{-1/3}_{bp}$. The concentration of bipolarons (i.e. Cooper pairs) $n_{bp}$ in the BCS is very large and for $T=0$ coincides with the concentration of charge carriers in metals.

In the above considered theory EPI is considered to be strong, therefore the correlation length is $l_{corr}<<n^{-1/3}_{bp}$. At the same time even at $T=0$ bipolarons are only a small part of charge carriers. This situation is realized in oxide ceramics. The notion of a pair in the TI-bipolaron theory under these conditions is well determined. Thus, according to [@2], the value of the correlation length for a TI bipolaron is $l_{corr}=\hbar^2\tilde{\epsilon}x(\eta)/e^2M_e$, where $x(\eta) (\eta=\epsilon_{\infty}/\epsilon_0)$ varies within $6\div10$ in the area of stability of bipolaron states. For the values of parameters corresponding to $YBCO$, it makes up $l_{corr}\approx10^{-7}$cm while $n_{bp}^{-1/3}\approx10^{-6}$ cm. Thus: $n_{bp}\,l_{corr}^3 \sim 10^{-3} \ll 1$, that is, individual pairs practically do not overlap.

The results obtained suggest that in order to raise the critical temperature $T_c$ one should either decrease the effective mass of charge carriers or increase the phonon frequency $\omega_0$, or else enhance the concentration of bipolarons $n_{bp}$. Hence, the problem of raising $T_c$ is related to the search for crystals with optimal parameter values. Notice that an increase in $\omega_0$ will not necessarily lead to an increase in $T_c$, since an increase in $\omega_0$ leads to a decrease in the EPI constant $\alpha$.

For small $\alpha$ we find ourselves in the field of applicability of the BCS which yields small $T_c$. This situation is probably realized in the anticorrelation dependence of $T_c$ on $\omega_0$ [@38].

The most effective way to change the concentration of $n_{bp}$ is to change the level of doping. In this case both
to be weak, accordingly, the correlation length, or the characteristic size of the couple is $ l_{corr}>>n^{-1/3}_{bp}$. The assiduity of bipolarons (i.e. Cooper copulate) $ n_{bp}$ in the BCS is very large and for $ T=0 $ coincides with the assiduity of charge carriers in metals. 

 In the above consider theory EPI is considered to be potent, therefore the correlation distance is $ l_{corr}<<n^{-1/3}_{bp}$. At the same time even at $ T=0 $ bipolarons are entirely a belittled part of charge carriers. This situation is realized in oxide ceramic. The notion of a pair in the TI - bipolaron theory under these condition is well determined. Thus, harmonize to [ @2 ], the value of the correlation duration for a TI bipolaron is $ l_{corr}=\hbar^2\tilde{\epsilon}x(\eta)/e^2M_e$, where $ x(\eta) (\eta=\epsilon_{\infty}/\epsilon_0)$ varies within $ 6\div10 $ in the area of stability of bipolaron states. For the values of argument corresponding to $ YBCO$, it makes up $ l_{corr}\approx10^{-7}$cm while $ n_{bp}^{-1/3}\approx10^{-6}$ cm. Thus: $ n_{bp}\,l_{corr}^3 \sim 10^{-3 } \ll 1 $, that is, individual pairs practically do not overlap. 

 The results obtained suggest that in order to raise the critical temperature $ T_c$ one should either decrease the effective mass of charge carriers or increase the phonon frequency $ \omega_0 $, or else enhance the concentration of bipolarons $ n_{bp}$. Hence, the problem of raising $ T_c$ is associate to the search for crystals with optimal argument value. comment that an increase in $ \omega_0 $ will not necessarily precede to an increase in $ T_c$, since an increase in $ \omega_0 $ leads to a decrease in the EPI constant $ \alpha$. 

 For belittled $ \alpha$ we find ourselves in the field of applicability of the BCS which yields small $ T_c$. This situation is probably realize in the anticorrelation dependence of $ T_c$ on $ \omega_0 $ [ @38 ]. 

 The most effective way to change the assiduity of $ n_{bp}$ is to change the horizontal surface of doping. In this shell both
 to be weak, accordingly, the correlation leutth, or the cgaracterkstic size of the pair is $l_{clre}>>n^{-1/3}_{bp}$. Uke concentration of cipolarond (i.e. Cooper kairs) $n_{bp}$ in the UDS is vcxy ladne anb hor $T=0$ coincides with the woncentration mf ckarge carriers in metals.

In the above considrrfd theory EPI ys cpgsidsgeb to be strong, therefore the codrelatimn length is $k_{corr}<<n^{-1/3}_{bp}$. At the same time fven at $T=0$ bipolarons age only a snall part of charee carriers. This situajion is realized in oxide ceramizs. Thz notion of a palt in the TI-bmpolarjn theory under thesa condiyions is well cetxrmibed. Thus, according to [@2], the value of the correlathou length for a TI bipilqron hs $l_{worr}=\fvar^2\gilse{\xpsjlon}x(\eha)/e^2J_e$, where $x(\sta) (\eta=\epsioon_{\infty}/\epsilon_0)$ varoef within $6\div10$ ih the wrqa of stability of bipolaron states. For ths values of parameters xorresponding to $YBCO$, it makes up $l_{corr}\approx10^{-7}$cm while $n_{bp}^{-1/3}\approx10^{-6}$ cm. Thus: $n_{bp}\,l_{cors}^3 \sim 10^{-3} \ll 1$, bhat us, individual pairs practically do not overlap.

Trs texults obtained suggest thst im order to raire the crjtical temperature $T_c$ one shouod either dectease the effective mass of charge carrpers or increase the pkonon frequeucy $\omgga_0$, or else enhance the conceutratikn of bipolwrons $n_{bp}$. Fence, the probleo on rdising $T_c$ is related to thq search hor cxystals dith optimwl parametfr values. Notice that an incrgase it $\omega_0$ wipl not necessarily lead to an iirrease in $T_c$, xitce an incrzase ik $\omega_0$ leads tj a decrease iu the EPN consgant $\alpha$.

Ror smanl $\alpha$ we find ourselvad in the fiend of ap[licqbiluty of gfe BCS which yoelds small $T_c$. This situation is probebly dealized in the anuixorrelation delenaense oh $T_c$ jt $\omega_0$ [@38].

The kost efwrctivd way to chcnee tne concentration of $t_{bp}$ js to change the lrvcl of dopung. In tris case both
to be weak, accordingly, the correlation length, characteristic of the is $l_{corr}>>n^{-1/3}_{bp}$. The pairs) in the BCS very large and $T=0$ coincides with the concentration of carriers in metals. In the above considered theory EPI is considered to be therefore the correlation length is $l_{corr}<<n^{-1/3}_{bp}$. At the same time even at $T=0$ are a part charge carriers. This situation is realized in oxide ceramics. The notion of a pair in the theory under these conditions is well determined. Thus, to [@2], the value the correlation length for a bipolaron $l_{corr}=\hbar^2\tilde{\epsilon}x(\eta)/e^2M_e$, where (\eta=\epsilon_{\infty}/\epsilon_0)$ within in the area stability of bipolaron states. For the values of parameters corresponding to $YBCO$, it makes up $l_{corr}\approx10^{-7}$cm while cm. Thus: 10^{-3} \ll that individual practically do not results obtained suggest that in order critical temperature $T_c$ one should either decrease the mass of carriers or increase the phonon frequency or else enhance the concentration of bipolarons $n_{bp}$. the problem of raising $T_c$ is related to the search for crystals with optimal parameter that an increase in will not necessarily to increase $T_c$, an increase $\omega_0$ leads to a decrease in the EPI constant $\alpha$. For $\alpha$ we find ourselves in the field of applicability of which small $T_c$. This is probably realized in anticorrelation of $T_c$ on $\omega_0$ most way concentration $n_{bp}$ to change the level doping. In this case both
 to be weak, accordingly, the corRelation leNgth, oR thE chArActeRistIc size of the paiR Is $l_{cOrr}>>n^{-1/3}_{bp}$. The concentration Of bipOlARons (I.E. COoper Pairs) $n_{bP}$ In THE BCs iS vEry LaRGe And foR $T=0$ cOincideS with the coNceNtRation of charGE cArriers in mEtaLs.

In the above ConSidereD tHeoRY EPI iS coNsideRed to bE Strong, Therefore ThE CorrelATion lenGTH iS $l_{coRr}<<n^{-1/3}_{bp}$. At the same timE EvEN at $T=0$ bipolarons Are onlY a SMaLL ParT of Charge carrIeRs. ThiS SituatiON iS REAliZEd in oxide ceraMics. The notiON of A pair iN tHe Ti-BipolaRon thEoRY unDer these conDitiOns is well DetermINed. Thus, ACcordinG to [@2], the ValUe oF the COrReLatIoN LenGTh For A tI bIpolaron Is $L_{cOrr}=\hbAr^2\tiLDE{\EPsilOn}x(\Eta)/e^2m_e$, wheRe $x(\eta) (\eta=\epsiLon_{\InftY}/\EpsIlon_0)$ vAries WithIn $6\Div10$ in The areA of stAbIlity of bipolaroN staTes. For the ValUeS of PaRametERs corrEspOndIng to $YBcO$, it makES up $L_{cORR}\ApProx10^{-7}$cm while $n_{bp}^{-1/3}\apprOx10^{-6}$ CM. thUs: $n_{bp}\,l_{coRr}^3 \sim 10^{-3} \lL 1$, ThAt IS, individUaL paIrs pRACticaLly dO NoT overlap.

the resULtS oBtained SuGgest tHaT in OrdEr to rAIse tHe critIcal tempEratuRE $T_c$ one should eiTHer decrease thE EfFECtIVe maSs oF charge carrIers OR incReasE ThE phONon frEquenCy $\OMeGA_0$, or else enhance the coNcEntratIon of Bipolarons $n_{bp}$. hence, the prOBLEm of raisIng $T_C$ Is RElated to the seaRch foR crystals wITh optimaL paraMeter valUes. Notice THAt an incrEasE in $\OmeGa_0$ wILL nOt necessarily LEAd to An IncreasE in $t_c$, since An iNcrEasE in $\OmEga_0$ leads tO a decreaSe In ThE EpI cOnstaNT $\alpha$.

FoR sMalL $\aLphA$ we fiND ourseLves iN the FiElD Of aPplicabILiTY Of thE BcS WhicH yiElDs smaLl $T_c$. tHis SituatiOn is probaBly REaliZeD iN the antIcorrelation dEpEndence of $T_C$ oN $\omEga_0$ [@38].

The MOSt effectIve way to change the concenTRation oF $n_{bP}$ is to ChanGe the leveL of Doping. in tHIs case Both
 to be weak, accordingly,the correl ation  le ngt h,  orthecharacteristic size  of the pair is $l_{co rr}>> n^ { -1/3 } _{ bp}$.  The co n ce n t rat io nofbi p ol arons  (i .e. Coo per pairs)  $n _{ bp}$ in theB CS  is very l arg e and for $T =0$  coinc id esw ith t heconce ntrati o n of c harge car ri e rs inm etals.I ntheabove consideredt he o ry EPI is cons idered  t o  b e str ong , therefor ethe c o rrelati o nl e n gth is $l_{corr}< <n^{-1/3}_{ b p}$ . At t he  sa m e time  even  a t  $T =0$ bipolar onsare onlya smal l  part o f  charge  carri ers . T hiss it ua tio ni s r e al ize d  in  oxide c er am ics.Then o t i on o f a  pai r inthe TI-bipola ron  the o ryunder  thes e co nd ition s is w ell d et ermined. Thus,acco rding to[@2 ],  th evalue of the  co rre lationlengthf oraT I bi polaron is $l_{cor r} = \ hb ar^2\til de{\ep s il on } x(\eta)/ e^ 2M_ e$,w h ere $ x(\e t a)  (\eta=\ epsilo n _{ \i nfty}/\ ep silon_ 0) $ v ari es wi t hin$6\div 10$ in t he ar e a of stability of bipolarons ta t e s. Forthe  values ofpara m eter s co r re spo n dingto $Y BC O $, it makes up $l_{cor r} \appro x10^{ -7}$cm while$n_{bp}^{- 1 / 3 }\approx 10^{ - 6} $  cm. Thus: $n_ {bp}\ ,l_{corr}^ 3  \sim 10 ^{-3}  \ll 1$,  that is, i ndividua l p air s p rac t i ca lly do not ov e r lap. 
The res ult s obtai ned  su gge stth at in ord er to ra is eth ecri tical temperat ur e $ T_ c$one s h ould e ither  dec re as e  th e effec t iv e mass  o fchar geca rrier s or inc rease t he phonon  fr e quen cy  $ \omega_ 0$, or else e nh ance the c on cen tratio n of bipol arons $n_{bp}$. Hence,t he prob lem  of r aisi ng $T_c$isrelate d t o  the s earchfor c ry sta l s  with o pt ima lparameterv a lue s. No ti ce t hat anincrease in $\omeg a _0$  will not nec ess aril y le adt oa n i nc r eas e in $T_c$, since  an increa se in  $\omega_0 $  le ad s to adecreas e int he EPIconstant$\alpha$. 
Fors m all  $\alpha$we findourselves in th e  f ieldofapplic ab ili ty of  the B C S w hichyields  s mall $ T_c$.  T his situ ation is probably reali zed in  theant icorrelat ion dep endence o f $T _c$ on $\o meg a_0 $ [@3 8]. 
Themost ef fec t ive w ay t o  change t h econ c e nt ration of $ n _ { bp} $ istoc hangethelevel of doping.I n this case bo th
 to_be weak,_accordingly, the correlation length,_or the_characteristic_size of_the_pair is $l_{corr}>>n^{-1/3}_{bp}$._The concentration of_bipolarons (i.e. Cooper pairs)_$n_{bp}$ in the_BCS_is very large and for $T=0$ coincides with the concentration of charge carriers in_metals.

In_the above_considered_theory_EPI is considered to be_strong, therefore the correlation length_is $l_{corr}<<n^{-1/3}_{bp}$._At the same time even at $T=0$ bipolarons_are_only a small_part of charge carriers. This situation is realized in_oxide ceramics. The notion of a_pair in the_TI-bipolaron_theory_under these conditions is_well determined. Thus, according to [@2],_the value of the correlation length_for a TI bipolaron is $l_{corr}=\hbar^2\tilde{\epsilon}x(\eta)/e^2M_e$, where_$x(\eta) (\eta=\epsilon_{\infty}/\epsilon_0)$ varies within $6\div10$ in_the area of stability of_bipolaron states._For the values of parameters_corresponding to $YBCO$,_it makes_up $l_{corr}\approx10^{-7}$cm while_$n_{bp}^{-1/3}\approx10^{-6}$ cm. Thus: $n_{bp}\,l_{corr}^3 \sim 10^{-3}_\ll 1$, that_is, individual pairs practically do not_overlap.

The_results obtained suggest_that_in_order to_raise the critical_temperature_$T_c$ one_should_either decrease the effective mass of_charge_carriers or increase the phonon frequency $\omega_0$,_or else enhance the_concentration_of bipolarons $n_{bp}$. Hence,_the problem of raising $T_c$_is related to the search for_crystals with_optimal parameter_values. Notice that an increase in $\omega_0$ will not necessarily lead_to an increase in $T_c$, since_an increase in $\omega_0$_leads to_a_decrease in the_EPI_constant $\alpha$.

For_small $\alpha$ we find ourselves in the_field of_applicability of the BCS which yields_small $T_c$. This situation_is_probably realized in the anticorrelation dependence_of $T_c$ on $\omega_0$ [@38].

The most_effective way to change the_concentration_of_$n_{bp}$ is to change the_level of doping. In this case_both